This product was designed for and is meant solely to be used by skilled professionals. Learn all warning statements and heed all really useful security precautions earlier than continuing.
DO NOT USE THIS SYSTEM WITHOUT SUFFICIENT VENTILATION. Customers should put on appropri- ate, correctly fitted NIOSH-approved activated charcoal cartridge respirator if a compelled fresh-air system is just not out there. All the time put on eye and face safety, in addition to gloves and protecting clothes. Don’t use this product, or be uncovered to spray mist / vapors when you have respiratory issues. KEEP OUT OF REACH OF CHILDREN AND PETS.
This method includes a number of elements. As soon as combined, this method can have hazards of all elements. Learn warnings on all packages earlier than opening.
Appropriate substrates embody:
– Eastwood Epoxy Primer
– Eastwood 2K Urethane Primer Surfacer
– Correctly ready manufacturing facility finishes
When portray over present finishes or cured undercoat merchandise:
– Clear floor with a Wax and Grease Remover, reminiscent of Eastwood’s 11999ZP, a powerful solvent mix designed to take away tar, wax, grease, highway grime, silicone and floor contaminants.
– Abrade floor to be painted with 320 grit sandpaper, ideally working as much as 600 grit for adhesion functions. Re-clean with a prep solvent to take away any particles earlier than software.
Apply single-stage urethane paints in two to a few medium moist coats as vital to realize ample protection, permitting ten minute flash between coats. Extra coats could also be vital to realize complete protection for some metallic colours. A ultimate “fog coat” could also be utilized with metallic colours to assist set a good flake sample and /or regulate flake orientation. A dry movie thickness of roughly 2 mil is really useful. Paint must be mud free inside 10-15 minutes and tack-free inside one hour (at 70 °F). Recoat anytime after the earlier coat has flashed, or earlier than 18 hours. After 18 hours, paint must be abraded previous to recoating for correct adhesion functions.
This urethane paint could also be utilized as a stand-along single-stage system, or together with Eastwood’s Excessive Solids Urethane Clear as a basecoat/clearcoat system. Moreover, Urethane Clear could also be built-in into Urethane coloration. When combining the 2 methods, make sure to activate either side (the paint and the clear) individually, with their very own activators at the right combination ratios, earlier than mixing.
Coating could also be compelled dry at 120°F for not less than 20 minutes, after a five-minute flash interval. Wait four-five hours after bake cycle to re-assemble.
When used as a Single-Stage Urethane Paint, this coating could also be wet-sanded and polished for elevated depth and gloss like some other urethane topcoat. Care must be taken when evenly reducing metallic colours to forestall disturbing aluminum flake.